# Electronic Supplementary Material (ESI) for CrystEngComm.
# This journal is © The Royal Society of Chemistry 2017

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_p
_database_code_depnum_ccdc_archive 'CCDC 1521983'
_audit_update_record             
;
2016-12-11 deposited with the CCDC.
2017-03-21 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'C24 H28 As3 Cu2 Mo18 N16 Na O64'
_chemical_formula_sum            'C24 H28 As3 Cu2 Mo18 N16 Na O64'
_chemical_formula_weight         3666.40

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           triclinic
_symmetry_space_group_name_H-M   'P -1'
_symmetry_space_group_name_Hall  '-P 1'
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   15.0907(9)
_cell_length_b                   15.2326(9)
_cell_length_c                   18.8918(11)
_cell_angle_alpha                80.9942(9)
_cell_angle_beta                 83.7204(10)
_cell_angle_gamma                75.2446(9)
_cell_volume                     4136.7(4)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    12548
_cell_measurement_theta_min      1.32
_cell_measurement_theta_max      25.73

_exptl_crystal_description       block
_exptl_crystal_colour            'dark blue'
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.18
_exptl_crystal_size_min          0.16
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    2.944
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             3440
_exptl_absorpt_coefficient_mu    4.401
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.477
_exptl_absorpt_correction_T_max  0.495
_exptl_absorpt_process_details   SADABS

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71000
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Bruker Smart APEX CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            20726
_diffrn_reflns_av_R_equivalents  0.0261
_diffrn_reflns_av_sigmaI/netI    0.0588
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_theta_min         1.39
_diffrn_reflns_theta_max         25.00
_reflns_number_total             14415
_reflns_number_gt                10357
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    SHELXP-97
_computing_publication_material  SHELXTL

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.1042P)²+104.5230P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         14415
_refine_ls_number_parameters     1138
_refine_ls_number_restraints     811
_refine_ls_R_factor_all          0.0820
_refine_ls_R_factor_gt           0.0757
_refine_ls_wR_factor_ref         0.1251
_refine_ls_wR_factor_gt          0.1037
_refine_ls_goodness_of_fit_ref   1.093
_refine_ls_restrained_S_all      1.099
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.13539(10) 0.56592(9) 0.76681(7) 0.0223(3) Uani 1 1 d U . .
Mo2 Mo 0.02883(9) 0.81577(9) 0.74644(7) 0.0210(3) Uani 1 1 d U . .
Mo3 Mo 0.35200(10) 0.87269(10) 0.53009(7) 0.0253(3) Uani 1 1 d U . .
Mo4 Mo 0.47266(10) 0.90784(10) 0.68012(7) 0.0247(3) Uani 1 1 d U . .
Mo5 Mo 0.57612(9) 0.68290(10) 0.69858(7) 0.0253(3) Uani 1 1 d U . .
Mo6 Mo 0.26135(9) 0.59902(9) 0.91573(7) 0.0208(3) Uani 1 1 d U . .
Mo7 Mo 0.45137(10) 0.64657(10) 0.55050(7) 0.0268(3) Uani 1 1 d U . .
Mo8 Mo 0.36948(10) 0.76458(11) 0.99567(7) 0.0264(3) Uani 1 1 d U . .
Mo9 Mo 0.46918(10) 0.91002(9) 0.87988(8) 0.0245(3) Uani 1 1 d U . .
Mo10 Mo 0.15403(9) 0.84694(10) 0.89846(7) 0.0231(3) Uani 1 1 d U . .
Mo11 Mo 0.25404(10) 0.99408(9) 0.78441(8) 0.0251(3) Uani 1 1 d U . .
Mo12 Mo 0.13130(10) 0.96307(9) 0.63127(8) 0.0250(3) Uani 1 1 d U . .
Mo13 Mo 0.57548(10) 0.68518(10) 0.89625(8) 0.0261(3) Uani 1 1 d U . .
Mo14 Mo 0.46441(9) 0.51973(9) 0.82239(7) 0.0216(3) Uani 1 1 d U . .
Mo15 Mo 0.33747(10) 0.48529(9) 0.67437(8) 0.0240(3) Uani 1 1 d U . .
Mo16 Mo 0.03629(10) 0.66594(10) 0.59024(8) 0.0276(3) Uani 1 1 d U . .
Mo17 Mo 0.14605(11) 0.81700(11) 0.47063(8) 0.0311(4) Uani 1 1 d U . .
Mo18 Mo 0.24247(11) 0.59035(10) 0.50191(8) 0.0309(4) Uani 1 1 d U . .
As2 As 0.4616(2) 0.5697(2) 0.98263(18) 0.0261(7) Uani 0.50 1 d PU . .
As3 As 0.23371(10) 0.72334(10) 0.64354(7) 0.0151(3) Uani 1 1 d U . .
As4 As 0.36795(10) 0.75957(10) 0.80534(8) 0.0145(3) Uani 1 1 d U . .
O1 O 0.0598(8) 0.5072(8) 0.8069(6) 0.033(3) Uani 1 1 d U . .
O2 O 0.3639(9) 0.9542(9) 0.4626(6) 0.043(3) Uani 1 1 d U . .
O3 O 0.6870(7) 0.6320(9) 0.6791(6) 0.034(3) Uani 1 1 d U . .
O4 O 0.3422(8) 0.7573(8) 1.0856(6) 0.033(3) Uani 1 1 d U . .
O5 O 0.5258(8) 0.5871(8) 0.7506(6) 0.029(3) Uani 1 1 d U . .
O6 O 0.5178(9) 0.9980(9) 0.6494(7) 0.042(3) Uani 1 1 d U . .
O7 O 0.0051(7) 0.7770(7) 0.6463(6) 0.026(2) Uani 1 1 d U . .
O8 O 0.6757(7) 0.6270(8) 0.9307(6) 0.030(3) Uani 1 1 d U . .
O9 O 0.6003(7) 0.6995(7) 0.8000(6) 0.025(2) Uani 1 1 d U . .
O10 O 0.5079(8) 0.9967(7) 0.9004(6) 0.032(3) Uani 1 1 d U . .
O11 O -0.0826(8) 0.8322(8) 0.7758(6) 0.033(3) Uani 1 1 d U . .
O12 O 0.3506(7) 0.6534(7) 0.8207(5) 0.020(2) Uani 1 1 d U . .
O13 O 0.5258(7) 0.6720(8) 0.6155(6) 0.028(3) Uani 1 1 d U . .
O14 O 0.5053(8) 0.9064(8) 0.7836(6) 0.030(3) Uani 1 1 d U . .
O15 O 0.5788(8) 0.8091(8) 0.6695(6) 0.032(3) Uani 1 1 d U . .
O16 O 0.0783(8) 0.5946(8) 0.6723(6) 0.029(3) Uani 1 1 d U . .
O17 O 0.4268(8) 0.8928(8) 0.5952(6) 0.030(3) Uani 1 1 d U . .
O18 O 0.1074(9) 0.8898(10) 0.3960(7) 0.046(3) Uani 1 1 d U . .
O19 O 0.5434(8) 0.4209(8) 0.8403(7) 0.036(3) Uani 1 1 d U . .
O20 O 0.5351(8) 0.5879(9) 0.4973(6) 0.037(3) Uani 1 1 d U . .
O21 O 0.2151(8) 0.5505(8) 0.9916(6) 0.031(3) Uani 1 1 d U . .
O22 O 0.2469(8) 0.9334(8) 0.5853(6) 0.030(3) Uani 1 1 d U . .
O23 O 0.0212(8) 0.9319(8) 0.6808(6) 0.035(3) Uani 1 1 d U . .
O24 O 0.0879(9) 1.0696(8) 0.5895(7) 0.040(3) Uani 1 1 d U . .
O25 O 0.2545(8) 0.8393(7) 0.4791(6) 0.027(3) Uani 1 1 d U . .
O26 O 0.3508(8) 0.9645(8) 0.7163(6) 0.030(3) Uani 1 1 d U . .
O27 O 0.1776(7) 0.7073(7) 0.5741(5) 0.022(2) Uani 1 1 d U . .
O28 O 0.5753(7) 0.8078(7) 0.9061(6) 0.026(2) Uani 1 1 d U . .
O29 O 0.3332(7) 0.7458(7) 0.6086(6) 0.024(2) Uani 1 1 d U . .
O30 O 0.1915(8) 0.7122(8) 0.4398(6) 0.040(3) Uani 1 1 d U . .
O31 O 0.4179(8) 0.8682(7) 0.9771(6) 0.027(3) Uani 1 1 d U . .
O32 O 0.0240(8) 0.7812(8) 0.5137(7) 0.039(3) Uani 1 1 d U . .
O33 O 0.4332(7) 0.7741(7) 0.7290(5) 0.022(2) Uani 1 1 d U . .
O34 O 0.2289(8) 0.4681(7) 0.7314(6) 0.027(2) Uani 1 1 d U . .
O35 O 0.3450(8) 0.6326(8) 0.4963(6) 0.029(3) Uani 1 1 d U . .
O36 O 0.4387(8) 0.7689(8) 0.4982(6) 0.030(3) Uani 1 1 d U . .
O37 O 0.2494(7) 0.6262(7) 0.7004(5) 0.021(2) Uani 1 1 d U . .
O38 O 0.1684(7) 0.8109(7) 0.6835(6) 0.024(2) Uani 1 1 d U . .
O39 O 0.1844(8) 0.7180(8) 0.9034(6) 0.028(3) Uani 1 1 d U . .
O40 O 0.3773(8) 0.5056(7) 0.9035(6) 0.028(3) Uani 1 1 d U . .
O41 O 0.1688(8) 0.9906(8) 0.7132(6) 0.029(3) Uani 1 1 d U . .
O42 O 0.4260(7) 0.7742(7) 0.8742(5) 0.019(2) Uani 1 1 d U . .
O43 O 0.0688(8) 0.8680(8) 0.9619(7) 0.037(3) Uani 1 1 d U . .
O44 O 0.2030(7) 0.5632(7) 0.8473(6) 0.026(2) Uani 1 1 d U . .
O45 O 0.2652(8) 0.5145(8) 0.5866(6) 0.030(3) Uani 1 1 d U . .
O46 O 0.3423(8) 0.6528(8) 0.9724(6) 0.029(3) Uani 1 1 d U . .
O47 O 0.0892(8) 0.8993(7) 0.5498(6) 0.027(3) Uani 1 1 d U . .
O48 O 0.1639(8) 0.9690(8) 0.8613(6) 0.034(3) Uani 1 1 d U . .
O49 O 0.4160(8) 0.5547(8) 0.6195(6) 0.028(3) Uani 1 1 d U . .
O50 O 0.4956(7) 0.6848(8) 0.9933(6) 0.029(3) Uani 1 1 d U . .
O51 O 0.2622(9) 0.5166(9) 0.4391(7) 0.044(3) Uani 1 1 d U . .
O52 O 0.3850(9) 0.3773(8) 0.6600(7) 0.036(3) Uani 1 1 d U . .
O53 O 0.3465(8) 0.9689(7) 0.8575(6) 0.028(3) Uani 1 1 d U . .
O54 O 0.2683(7) 0.8392(7) 0.8061(6) 0.024(2) Uani 1 1 d U . .
O55 O 0.3982(7) 0.4873(7) 0.7579(6) 0.026(2) Uani 1 1 d U . .
O56 O 0.5173(7) 0.5864(7) 0.8910(6) 0.025(2) Uani 1 1 d U . .
O57 O 0.2303(9) 1.1081(8) 0.7781(7) 0.039(3) Uani 1 1 d U . .
O58 O 0.0748(8) 0.8529(8) 0.8189(6) 0.028(3) Uani 1 1 d U . .
O59 O -0.0694(9) 0.6503(9) 0.5858(7) 0.042(3) Uani 1 1 d U . .
O60 O 0.1075(8) 0.5936(8) 0.5295(7) 0.039(3) Uani 1 1 d U . .
O61 O 0.2548(7) 0.8317(7) 0.9600(6) 0.026(2) Uani 1 1 d U . .
O62 O 0.0762(8) 0.6920(8) 0.7731(6) 0.028(3) Uani 1 1 d U . .
Cu1 Cu 0.0641(2) 0.6028(3) 0.0875(2) 0.0823(11) Uani 1 1 d U . .
N11 N -0.0199(12) 0.6204(12) 0.0179(9) 0.050(4) Uani 1 1 d U . .
N12 N -0.1425(13) 0.6181(13) -0.0334(10) 0.056(5) Uani 1 1 d U . .
N9 N 0.1392(16) 0.5867(16) 0.1615(12) 0.074(6) Uani 1 1 d U . .
N10 N 0.2585(16) 0.5676(16) 0.2265(13) 0.076(6) Uani 1 1 d U . .
C7 C 0.112(2) 0.595(2) 0.2334(18) 0.096(10) Uani 1 1 d U . .
H7 H 0.0507 0.6102 0.2517 0.115 Uiso 1 1 calc R . .
C9 C 0.228(2) 0.5748(19) 0.1601(16) 0.076(8) Uani 1 1 d U . .
H9 H 0.2660 0.5715 0.1181 0.091 Uiso 1 1 calc R . .
C11 C -0.0878(15) 0.6544(15) -0.0827(12) 0.050(5) Uani 1 1 d U . .
H11 H -0.0991 0.6738 -0.1308 0.060 Uiso 1 1 calc R . .
C10 C -0.1007(16) 0.5968(16) 0.0290(13) 0.059(6) Uani 1 1 d U . .
H10 H -0.1241 0.5703 0.0723 0.070 Uiso 1 1 calc R . .
C12 C -0.0139(17) 0.6585(17) -0.0519(14) 0.064(6) Uani 1 1 d U . .
H12 H 0.0338 0.6833 -0.0744 0.077 Uiso 1 1 calc R . .
C8 C 0.184(2) 0.580(2) 0.272(2) 0.104(11) Uani 1 1 d U . .
H8 H 0.1822 0.5782 0.3220 0.125 Uiso 1 1 calc R . .
Cu2 Cu 0.2114(2) 0.28744(19) 0.76152(14) 0.0528(7) Uani 1 1 d U . .
N4 N 0.2876(11) 0.2722(10) 0.8362(8) 0.037(4) Uani 1 1 d U . .
N2 N 0.1359(12) 0.3031(11) 0.6848(9) 0.046(4) Uani 1 1 d U . .
N1 N 0.0557(13) 0.2754(13) 0.6043(10) 0.053(5) Uani 1 1 d U . .
N3 N 0.3737(11) 0.3002(10) 0.9115(8) 0.038(4) Uani 1 1 d U . .
C20 C 0.3875(16) 0.2071(15) 0.9209(12) 0.053(5) Uani 1 1 d U . .
H20 H 0.4255 0.1642 0.9521 0.063 Uiso 1 1 calc R . .
C22 C 0.0515(16) 0.3662(16) 0.5918(12) 0.055(6) Uani 1 1 d U . .
H22 H 0.0183 0.4084 0.5573 0.067 Uiso 1 1 calc R . .
C19 C 0.3343(16) 0.1921(17) 0.8754(13) 0.059(6) Uani 1 1 d U . .
H19 H 0.3286 0.1341 0.8701 0.071 Uiso 1 1 calc R . .
C24 C 0.1113(15) 0.2384(15) 0.6595(11) 0.049(5) Uani 1 1 d U . .
H24 H 0.1289 0.1763 0.6765 0.059 Uiso 1 1 calc R . .
C21 C 0.3141(12) 0.3361(12) 0.8609(9) 0.033(4) Uani 1 1 d U . .
H21 H 0.2942 0.3984 0.8455 0.040 Uiso 1 1 calc R . .
C23 C 0.1042(14) 0.3849(14) 0.6383(11) 0.045(5) Uani 1 1 d U . .
H23 H 0.1172 0.4411 0.6394 0.054 Uiso 1 1 calc R . .
Na1 Na 0.0559(5) 1.0969(5) 0.9334(4) 0.0316(8) Uani 1 1 d DU . .
N6 N 0.2251(16) 1.0891(15) 1.0964(12) 0.073(6) Uani 1 1 d U . .
N5 N 0.1531(18) 1.0622(18) 1.0072(14) 0.079(5) Uani 1 1 d U . .
C15 C 0.140(2) 1.100(2) 1.0712(17) 0.087(9) Uani 1 1 d U . .
H15 H 0.0841 1.1276 1.0931 0.105 Uiso 1 1 calc R . .
C14 C 0.2857(19) 1.0397(18) 1.0521(14) 0.067(7) Uani 1 1 d U . .
H14 H 0.3488 1.0225 1.0567 0.080 Uiso 1 1 calc R . .
C13 C 0.2476(11) 1.0196(14) 1.0044(11) 0.046(5) Uani 1 1 d DU . .
H13 H 0.2776 0.9812 0.9709 0.055 Uiso 1 1 calc R . .
O2W O 0.6021(12) 0.4397(12) 0.6653(9) 0.078(5) Uani 1 1 d U . .
H2WA H 0.6421 0.4596 0.6366 0.093 Uiso 1 1 d R . .
H2WB H 0.6150 0.3850 0.6866 0.093 Uiso 1 1 d R . .
O1W O 0.2800(13) 0.1500(19) 0.2142(10) 0.115(9) Uani 1 1 d U . .
H1WA H 0.3202 0.1610 0.1811 0.138 Uiso 1 1 d R . .
H1WB H 0.2495 0.1114 0.2105 0.138 Uiso 1 1 d R . .
N1B N 0.5822(16) 0.2715(16) 0.7127(13) 0.078(6) Uani 1 1 d U . .
N1C N 0.581(2) 0.149(2) 0.6844(17) 0.112(9) Uani 1 1 d U . .
C3 C 0.597(2) 0.226(2) 0.6624(19) 0.097(10) Uani 1 1 d U . .
H3 H 0.6159 0.2459 0.6155 0.117 Uiso 1 1 calc R . .
C2 C 0.558(3) 0.225(3) 0.774(2) 0.108(11) Uani 1 1 d U . .
H2 H 0.5442 0.2451 0.8183 0.130 Uiso 1 1 calc R . .
C1 C 0.558(3) 0.146(3) 0.759(2) 0.126(13) Uani 1 1 d U . .
H1 H 0.5454 0.0966 0.7910 0.151 Uiso 1 1 calc R . .
C6 C 0.7234(16) 0.7008(15) 0.5065(12) 0.096(10) Uani 1 1 d GU . .
H6 H 0.7538 0.6495 0.5358 0.115 Uiso 1 1 calc R . .
N1G N 0.6713(18) 0.7003(17) 0.4484(14) 0.127(11) Uani 1 1 d GU . .
C5 C 0.6365(18) 0.793(2) 0.4181(13) 0.140(15) Uani 1 1 d GU . .
H5 H 0.6001 0.8120 0.3792 0.168 Uiso 1 1 calc R . .
C4 C 0.667(2) 0.8500(13) 0.4575(16) 0.150(17) Uani 1 1 d GU . .
H4 H 0.6542 0.9136 0.4489 0.180 Uiso 1 1 calc R . .
N1D N 0.7208(17) 0.7933(18) 0.5121(13) 0.123(10) Uani 1 1 d GU . .
N7 N -0.055(2) 1.122(2) 0.8693(12) 0.133(5) Uani 1 1 d GU . .
C18 C -0.149(2) 1.163(2) 0.8614(16) 0.160(18) Uani 1 1 d GU . .
H18 H -0.1891 1.1983 0.8931 0.192 Uiso 1 1 calc R . .
C17 C -0.1725(15) 1.141(2) 0.7966(18) 0.19(2) Uani 1 1 d GU . .
H17 H -0.2301 1.1591 0.7785 0.223 Uiso 1 1 calc R . .
N8 N -0.0921(19) 1.0862(17) 0.7645(11) 0.103(6) Uani 1 1 d GU . .
C16 C -0.0193(14) 1.0746(17) 0.8094(14) 0.089(6) Uani 1 1 d GU . .
H16 H 0.0410 1.0416 0.8010 0.106 Uiso 1 1 calc R . .
As1 As -0.0202(3) 0.8749(3) 0.5740(2) 0.0316(8) Uani 0.50 1 d PU . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O1 1.671(11) . ?
Mo1 O44 1.911(11) . ?
Mo1 O62 1.917(11) . ?
Mo1 O34 1.922(11) . ?
Mo1 O16 2.006(11) . ?
Mo1 O37 2.312(10) . ?
Mo2 O11 1.680(11) . ?
Mo2 O58 1.824(11) . ?
Mo2 O62 1.848(11) . ?
Mo2 O23 1.980(12) . ?
Mo2 O7 2.160(10) . ?
Mo2 O38 2.293(11) . ?
Mo3 O2 1.663(12) . ?
Mo3 O17 1.866(11) . ?
Mo3 O36 1.910(11) . ?
Mo3 O22 1.911(11) . ?
Mo3 O25 2.049(11) . ?
Mo3 O29 2.303(11) . ?
Mo4 O6 1.681(12) . ?
Mo4 O17 1.882(11) . ?
Mo4 O15 1.915(12) . ?
Mo4 O26 1.922(11) . ?
Mo4 O14 2.063(11) . ?
Mo4 O33 2.295(10) . ?
Mo5 O3 1.682(11) . ?
Mo5 O13 1.863(11) . ?
Mo5 O5 1.904(11) . ?
Mo5 O15 1.924(12) . ?
Mo5 O9 2.054(10) . ?
Mo5 O33 2.316(10) . ?
Mo6 O21 1.673(11) . ?
Mo6 O44 1.860(11) . ?
Mo6 O39 1.882(11) . ?
Mo6 O40 1.971(11) . ?
Mo6 O46 2.093(11) . ?
Mo6 O12 2.302(10) . ?
Mo7 O20 1.683(11) . ?
Mo7 O13 1.896(11) . ?
Mo7 O49 1.898(11) . ?
Mo7 O36 1.941(11) . ?
Mo7 O35 2.067(11) . ?
Mo7 O29 2.321(10) . ?
Mo8 O4 1.697(11) . ?
Mo8 O31 1.873(11) . ?
Mo8 O61 1.906(11) . ?
Mo8 O46 1.972(11) . ?
Mo8 O50 1.981(11) . ?
Mo8 O42 2.355(10) . ?
Mo8 As2 2.976(4) . ?
Mo9 O10 1.684(11) . ?
Mo9 O14 1.846(11) . ?
Mo9 O53 1.902(11) . ?
Mo9 O28 1.974(11) . ?
Mo9 O31 1.988(11) . ?
Mo9 O42 2.344(10) . ?
Mo10 O43 1.664(12) . ?
Mo10 O39 1.890(11) . ?
Mo10 O48 1.918(12) . ?
Mo10 O61 1.960(11) . ?
Mo10 O58 1.998(11) . ?
Mo10 O54 2.310(11) . ?
Mo11 O57 1.669(11) . ?
Mo11 O26 1.851(11) . ?
Mo11 O48 1.940(12) . ?
Mo11 O41 1.975(11) . ?
Mo11 O53 1.996(11) . ?
Mo11 O54 2.289(11) . ?
Mo12 O24 1.690(11) . ?
Mo12 O22 1.842(11) . ?
Mo12 O41 1.847(11) . ?
Mo12 O23 1.945(12) . ?
Mo12 O47 2.170(11) . ?
Mo12 O38 2.324(10) . ?
Mo13 O8 1.688(11) . ?
Mo13 O9 1.807(10) . ?
Mo13 O28 1.906(11) . ?
Mo13 O56 1.946(11) . ?
Mo13 O50 2.081(11) . ?
Mo13 O42 2.361(10) . ?
Mo13 As2 2.956(4) . ?
Mo14 O19 1.677(11) . ?
Mo14 O55 1.853(11) . ?
Mo14 O5 1.877(11) . ?
Mo14 O40 1.930(11) . ?
Mo14 O56 2.097(11) . ?
Mo14 O12 2.304(10) . ?
Mo15 O52 1.671(11) . ?
Mo15 O49 1.903(11) . ?
Mo15 O34 1.912(11) . ?
Mo15 O55 1.918(11) . ?
Mo15 O45 2.014(11) . ?
Mo15 O37 2.313(10) . ?
Mo16 O59 1.684(13) . ?
Mo16 O60 1.792(12) . ?
Mo16 O16 1.822(11) . ?
Mo16 O7 2.062(10) . ?
Mo16 O32 2.076(12) . ?
Mo16 O27 2.350(10) . ?
Mo16 As1 3.053(5) . ?
Mo17 O18 1.709(12) . ?
Mo17 O30 1.733(12) . ?
Mo17 O25 1.782(11) . ?
Mo17 O47 2.075(11) . ?
Mo17 O32 2.096(12) . ?
Mo17 O27 2.370(10) . ?
Mo17 As1 3.038(5) . ?
Mo18 O51 1.712(12) . ?
Mo18 O35 1.807(12) . ?
Mo18 O45 1.830(11) . ?
Mo18 O60 2.037(12) . ?
Mo18 O30 2.050(11) . ?
Mo18 O27 2.361(10) . ?
As2 O56 1.850(11) . ?
As2 O46 1.928(12) . ?
As2 O50 1.993(12) . ?
As2 As2 2.182(7) 2_667 ?
As3 O37 1.668(10) . ?
As3 O29 1.668(11) . ?
As3 O38 1.674(10) . ?
As3 O27 1.716(10) . ?
As4 O33 1.673(10) . ?
As4 O54 1.674(11) . ?
As4 O12 1.679(10) . ?
As4 O42 1.716(10) . ?
O7 As1 1.849(12) . ?
O32 As1 1.907(14) . ?
O43 Na1 2.597(14) 2_577 ?
O47 As1 1.780(12) . ?
O48 Na1 2.653(14) . ?
Cu1 N9 1.84(2) . ?
Cu1 N11 1.868(17) . ?
N11 C10 1.34(3) . ?
N11 C12 1.36(3) . ?
N12 C11 1.33(3) . ?
N12 C10 1.35(3) . ?
N9 C9 1.30(3) . ?
N9 C7 1.39(4) . ?
N10 C8 1.34(4) . ?
N10 C9 1.36(3) . ?
C7 C8 1.33(4) . ?
C7 H7 0.9300 . ?
C9 H9 0.9300 . ?
C11 C12 1.33(3) . ?
C11 H11 0.9300 . ?
C10 H10 0.9300 . ?
C12 H12 0.9300 . ?
C8 H8 0.9300 . ?
Cu2 N4 1.866(15) . ?
Cu2 N2 1.889(17) . ?
N4 C21 1.31(2) . ?
N4 C19 1.39(3) . ?
N2 C24 1.31(2) . ?
N2 C23 1.41(3) . ?
N1 C22 1.35(3) . ?
N1 C24 1.37(3) . ?
N3 C21 1.34(2) . ?
N3 C20 1.37(3) . ?
C20 C19 1.32(3) . ?
C20 H20 0.9300 . ?
C22 C23 1.35(3) . ?
C22 H22 0.9300 . ?
C19 H19 0.9300 . ?
C24 H24 0.9300 . ?
C21 H21 0.9300 . ?
C23 H23 0.9300 . ?
Na1 N5 2.05(3) . ?
Na1 N7 2.09(3) . ?
Na1 O43 2.597(14) 2_577 ?
Na1 Na1 4.145(16) 2_577 ?
N6 C14 1.34(3) . ?
N6 C15 1.38(4) . ?
N5 C15 1.39(4) . ?
N5 C13 1.41(3) . ?
C15 H15 0.9300 . ?
C14 C13 1.24(3) . ?
C14 H14 0.9300 . ?
C13 H13 0.9300 . ?
O2W H2WA 0.8500 . ?
O2W H2WB 0.8500 . ?
O1W H1WA 0.8500 . ?
O1W H1WB 0.8500 . ?
N1B C3 1.23(4) . ?
N1B C2 1.32(4) . ?
N1C C3 1.25(4) . ?
N1C C1 1.42(5) . ?
C3 H3 0.9300 . ?
C2 C1 1.27(5) . ?
C2 H2 0.9300 . ?
C1 H1 0.9300 . ?
C6 N1G 1.4200 . ?
C6 N1D 1.4200 . ?
C6 H6 0.9300 . ?
N1G C5 1.4200 . ?
C5 C4 1.4200 . ?
C5 H5 0.9300 . ?
C4 N1D 1.4200 . ?
C4 H4 0.9300 . ?
N7 C16 1.4200 . ?
N7 C18 1.4200 . ?
C18 C17 1.4200 . ?
C18 H18 0.9300 . ?
C17 N8 1.4200 . ?
C17 H17 0.9300 . ?
N8 C16 1.4200 . ?
C16 H16 0.9300 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 Mo1 O44 99.3(5) . . ?
O1 Mo1 O62 105.2(6) . . ?
O44 Mo1 O62 89.7(5) . . ?
O1 Mo1 O34 100.0(6) . . ?
O44 Mo1 O34 91.7(5) . . ?
O62 Mo1 O34 154.2(5) . . ?
O1 Mo1 O16 94.1(5) . . ?
O44 Mo1 O16 165.8(5) . . ?
O62 Mo1 O16 82.4(5) . . ?
O34 Mo1 O16 90.4(5) . . ?
O1 Mo1 O37 170.2(5) . . ?
O44 Mo1 O37 84.7(4) . . ?
O62 Mo1 O37 83.6(4) . . ?
O34 Mo1 O37 70.9(4) . . ?
O16 Mo1 O37 82.7(4) . . ?
O11 Mo2 O58 100.7(5) . . ?
O11 Mo2 O62 103.7(6) . . ?
O58 Mo2 O62 95.5(5) . . ?
O11 Mo2 O23 98.5(6) . . ?
O58 Mo2 O23 95.1(5) . . ?
O62 Mo2 O23 153.1(5) . . ?
O11 Mo2 O7 92.6(5) . . ?
O58 Mo2 O7 166.0(5) . . ?
O62 Mo2 O7 85.5(4) . . ?
O23 Mo2 O7 78.4(5) . . ?
O11 Mo2 O38 167.5(5) . . ?
O58 Mo2 O38 87.4(4) . . ?
O62 Mo2 O38 84.7(4) . . ?
O23 Mo2 O38 71.1(4) . . ?
O7 Mo2 O38 78.7(4) . . ?
O2 Mo3 O17 100.6(6) . . ?
O2 Mo3 O36 101.2(6) . . ?
O17 Mo3 O36 95.4(5) . . ?
O2 Mo3 O22 102.0(6) . . ?
O17 Mo3 O22 89.0(5) . . ?
O36 Mo3 O22 155.1(5) . . ?
O2 Mo3 O25 90.9(5) . . ?
O17 Mo3 O25 167.1(5) . . ?
O36 Mo3 O25 88.1(5) . . ?
O22 Mo3 O25 82.8(5) . . ?
O2 Mo3 O29 170.3(5) . . ?
O17 Mo3 O29 87.6(4) . . ?
O36 Mo3 O29 72.7(4) . . ?
O22 Mo3 O29 83.1(4) . . ?
O25 Mo3 O29 81.5(4) . . ?
O6 Mo4 O17 99.7(5) . . ?
O6 Mo4 O15 100.4(6) . . ?
O17 Mo4 O15 92.4(5) . . ?
O6 Mo4 O26 102.9(6) . . ?
O17 Mo4 O26 90.6(5) . . ?
O15 Mo4 O26 155.6(5) . . ?
O6 Mo4 O14 92.1(5) . . ?
O17 Mo4 O14 167.8(5) . . ?
O15 Mo4 O14 88.5(5) . . ?
O26 Mo4 O14 83.7(5) . . ?
O6 Mo4 O33 171.0(5) . . ?
O17 Mo4 O33 86.0(4) . . ?
O15 Mo4 O33 72.2(4) . . ?
O26 Mo4 O33 83.9(4) . . ?
O14 Mo4 O33 82.7(4) . . ?
O3 Mo5 O13 99.9(5) . . ?
O3 Mo5 O5 104.4(6) . . ?
O13 Mo5 O5 90.5(5) . . ?
O3 Mo5 O15 99.9(6) . . ?
O13 Mo5 O15 94.5(5) . . ?
O5 Mo5 O15 154.0(5) . . ?
O3 Mo5 O9 92.8(5) . . ?
O13 Mo5 O9 166.6(4) . . ?
O5 Mo5 O9 82.2(4) . . ?
O15 Mo5 O9 87.5(5) . . ?
O3 Mo5 O33 170.0(5) . . ?
O13 Mo5 O33 86.1(4) . . ?
O5 Mo5 O33 83.3(4) . . ?
O15 Mo5 O33 71.6(4) . . ?
O9 Mo5 O33 82.0(4) . . ?
O21 Mo6 O44 100.9(5) . . ?
O21 Mo6 O39 102.8(5) . . ?
O44 Mo6 O39 91.2(5) . . ?
O21 Mo6 O40 100.1(5) . . ?
O44 Mo6 O40 94.8(5) . . ?
O39 Mo6 O40 154.8(5) . . ?
O21 Mo6 O46 92.1(5) . . ?
O44 Mo6 O46 167.0(5) . . ?
O39 Mo6 O46 86.4(5) . . ?
O40 Mo6 O46 82.3(4) . . ?
O21 Mo6 O12 169.3(5) . . ?
O44 Mo6 O12 86.2(4) . . ?
O39 Mo6 O12 84.9(4) . . ?
O40 Mo6 O12 71.2(4) . . ?
O46 Mo6 O12 80.8(4) . . ?
O20 Mo7 O13 98.7(5) . . ?
O20 Mo7 O49 104.2(6) . . ?
O13 Mo7 O49 91.5(5) . . ?
O20 Mo7 O36 99.5(6) . . ?
O13 Mo7 O36 90.6(5) . . ?
O49 Mo7 O36 155.5(5) . . ?
O20 Mo7 O35 94.9(5) . . ?
O13 Mo7 O35 166.3(4) . . ?
O49 Mo7 O35 83.7(5) . . ?
O36 Mo7 O35 88.6(5) . . ?
O20 Mo7 O29 170.9(5) . . ?
O13 Mo7 O29 84.2(4) . . ?
O49 Mo7 O29 84.2(4) . . ?
O36 Mo7 O29 71.8(4) . . ?
O35 Mo7 O29 82.5(4) . . ?
O4 Mo8 O31 102.4(5) . . ?
O4 Mo8 O61 100.9(5) . . ?
O31 Mo8 O61 92.1(5) . . ?
O4 Mo8 O46 102.1(5) . . ?
O31 Mo8 O46 155.0(5) . . ?
O61 Mo8 O46 88.0(5) . . ?
O4 Mo8 O50 100.6(5) . . ?
O31 Mo8 O50 89.9(5) . . ?
O61 Mo8 O50 157.5(4) . . ?
O46 Mo8 O50 80.9(5) . . ?
O4 Mo8 O42 172.9(5) . . ?
O31 Mo8 O42 73.7(4) . . ?
O61 Mo8 O42 85.3(4) . . ?
O46 Mo8 O42 81.4(4) . . ?
O50 Mo8 O42 73.7(4) . . ?
O4 Mo8 As2 100.3(4) . . ?
O31 Mo8 As2 129.6(4) . . ?
O61 Mo8 As2 126.7(3) . . ?
O46 Mo8 As2 39.7(3) . . ?
O50 Mo8 As2 41.7(3) . . ?
O42 Mo8 As2 78.4(3) . . ?
O10 Mo9 O14 104.1(6) . . ?
O10 Mo9 O53 102.4(5) . . ?
O14 Mo9 O53 90.8(5) . . ?
O10 Mo9 O28 98.9(5) . . ?
O14 Mo9 O28 90.5(5) . . ?
O53 Mo9 O28 157.7(5) . . ?
O10 Mo9 O31 98.8(5) . . ?
O14 Mo9 O31 156.9(5) . . ?
O53 Mo9 O31 87.4(5) . . ?
O28 Mo9 O31 82.8(5) . . ?
O10 Mo9 O42 168.2(5) . . ?
O14 Mo9 O42 84.8(4) . . ?
O53 Mo9 O42 84.9(4) . . ?
O28 Mo9 O42 73.0(4) . . ?
O31 Mo9 O42 72.1(4) . . ?
O43 Mo10 O39 103.7(5) . . ?
O43 Mo10 O48 100.9(6) . . ?
O39 Mo10 O48 155.4(5) . . ?
O43 Mo10 O61 96.8(5) . . ?
O39 Mo10 O61 87.1(5) . . ?
O48 Mo10 O61 90.7(5) . . ?
O43 Mo10 O58 96.3(5) . . ?
O39 Mo10 O58 88.2(5) . . ?
O48 Mo10 O58 88.4(5) . . ?
O61 Mo10 O58 166.8(4) . . ?
O43 Mo10 O54 172.2(5) . . ?
O39 Mo10 O54 84.1(4) . . ?
O48 Mo10 O54 71.3(4) . . ?
O61 Mo10 O54 84.4(4) . . ?
O58 Mo10 O54 82.9(4) . . ?
O57 Mo11 O26 104.5(6) . . ?
O57 Mo11 O48 99.9(6) . . ?
O26 Mo11 O48 155.6(5) . . ?
O57 Mo11 O41 95.7(5) . . ?
O26 Mo11 O41 88.8(5) . . ?
O48 Mo11 O41 89.6(5) . . ?
O57 Mo11 O53 96.3(5) . . ?
O26 Mo11 O53 87.9(5) . . ?
O48 Mo11 O53 88.6(5) . . ?
O41 Mo11 O53 167.9(5) . . ?
O57 Mo11 O54 171.3(5) . . ?
O26 Mo11 O54 84.1(4) . . ?
O48 Mo11 O54 71.5(4) . . ?
O41 Mo11 O54 84.0(4) . . ?
O53 Mo11 O54 84.1(4) . . ?
O24 Mo12 O22 102.0(6) . . ?
O24 Mo12 O41 100.5(5) . . ?
O22 Mo12 O41 95.9(5) . . ?
O24 Mo12 O23 101.5(6) . . ?
O22 Mo12 O23 152.7(5) . . ?
O41 Mo12 O23 93.4(5) . . ?
O24 Mo12 O47 92.4(5) . . ?
O22 Mo12 O47 85.5(5) . . ?
O41 Mo12 O47 166.4(5) . . ?
O23 Mo12 O47 79.8(5) . . ?
O24 Mo12 O38 170.2(5) . . ?
O22 Mo12 O38 83.9(4) . . ?
O41 Mo12 O38 86.5(4) . . ?
O23 Mo12 O38 71.0(4) . . ?
O47 Mo12 O38 80.2(4) . . ?
O8 Mo13 O9 105.4(5) . . ?
O8 Mo13 O28 101.1(5) . . ?
O9 Mo13 O28 94.5(5) . . ?
O8 Mo13 O56 101.6(5) . . ?
O9 Mo13 O56 91.2(5) . . ?
O28 Mo13 O56 154.1(5) . . ?
O8 Mo13 O50 96.4(5) . . ?
O9 Mo13 O50 157.6(5) . . ?
O28 Mo13 O50 86.1(5) . . ?
O56 Mo13 O50 79.3(4) . . ?
O8 Mo13 O42 167.3(5) . . ?
O9 Mo13 O42 86.7(4) . . ?
O28 Mo13 O42 73.8(4) . . ?
O56 Mo13 O42 81.4(4) . . ?
O50 Mo13 O42 71.9(4) . . ?
O8 Mo13 As2 96.1(4) . . ?
O9 Mo13 As2 128.1(3) . . ?
O28 Mo13 As2 127.2(3) . . ?
O56 Mo13 As2 37.7(3) . . ?
O50 Mo13 As2 42.3(3) . . ?
O42 Mo13 As2 78.7(3) . . ?
O19 Mo14 O55 100.4(5) . . ?
O19 Mo14 O5 103.1(6) . . ?
O55 Mo14 O5 93.7(5) . . ?
O19 Mo14 O40 99.0(6) . . ?
O55 Mo14 O40 94.8(5) . . ?
O5 Mo14 O40 154.5(5) . . ?
O19 Mo14 O56 93.1(5) . . ?
O55 Mo14 O56 166.5(4) . . ?
O5 Mo14 O56 83.0(4) . . ?
O40 Mo14 O56 83.1(4) . . ?
O19 Mo14 O12 169.3(5) . . ?
O55 Mo14 O12 86.1(4) . . ?
O5 Mo14 O12 84.8(4) . . ?
O40 Mo14 O12 71.8(4) . . ?
O56 Mo14 O12 80.6(4) . . ?
O52 Mo15 O49 104.7(6) . . ?
O52 Mo15 O34 99.6(6) . . ?
O49 Mo15 O34 155.4(5) . . ?
O52 Mo15 O55 99.2(5) . . ?
O49 Mo15 O55 88.5(5) . . ?
O34 Mo15 O55 91.9(5) . . ?
O52 Mo15 O45 93.7(5) . . ?
O49 Mo15 O45 85.5(5) . . ?
O34 Mo15 O45 88.8(5) . . ?
O55 Mo15 O45 166.8(4) . . ?
O52 Mo15 O37 170.3(5) . . ?
O49 Mo15 O37 84.5(4) . . ?
O34 Mo15 O37 71.0(4) . . ?
O55 Mo15 O37 84.0(4) . . ?
O45 Mo15 O37 83.8(4) . . ?
O59 Mo16 O60 103.9(6) . . ?
O59 Mo16 O16 105.1(6) . . ?
O60 Mo16 O16 96.1(6) . . ?
O59 Mo16 O7 100.6(5) . . ?
O60 Mo16 O7 153.1(5) . . ?
O16 Mo16 O7 88.0(5) . . ?
O59 Mo16 O32 96.9(6) . . ?
O60 Mo16 O32 92.4(6) . . ?
O16 Mo16 O32 153.7(5) . . ?
O7 Mo16 O32 73.7(5) . . ?
O59 Mo16 O27 168.3(5) . . ?
O60 Mo16 O27 74.1(5) . . ?
O16 Mo16 O27 86.6(4) . . ?
O7 Mo16 O27 79.7(4) . . ?
O32 Mo16 O27 71.8(4) . . ?
O59 Mo16 As1 96.5(5) . . ?
O60 Mo16 As1 128.6(4) . . ?
O16 Mo16 As1 123.4(4) . . ?
O7 Mo16 As1 36.2(3) . . ?
O32 Mo16 As1 38.0(4) . . ?
O27 Mo16 As1 76.7(3) . . ?
O18 Mo17 O30 104.4(6) . . ?
O18 Mo17 O25 103.3(6) . . ?
O30 Mo17 O25 95.2(6) . . ?
O18 Mo17 O47 100.2(6) . . ?
O30 Mo17 O47 153.4(5) . . ?
O25 Mo17 O47 88.9(5) . . ?
O18 Mo17 O32 100.0(6) . . ?
O30 Mo17 O32 93.0(6) . . ?
O25 Mo17 O32 152.4(5) . . ?
O47 Mo17 O32 72.6(5) . . ?
O18 Mo17 O27 170.6(5) . . ?
O30 Mo17 O27 73.7(4) . . ?
O25 Mo17 O27 86.1(4) . . ?
O47 Mo17 O27 80.3(4) . . ?
O32 Mo17 O27 71.1(4) . . ?
O18 Mo17 As1 98.2(5) . . ?
O30 Mo17 As1 129.6(4) . . ?
O25 Mo17 As1 122.5(4) . . ?
O47 Mo17 As1 34.7(3) . . ?
O32 Mo17 As1 38.4(4) . . ?
O27 Mo17 As1 76.8(3) . . ?
O51 Mo18 O35 105.7(6) . . ?
O51 Mo18 O45 103.7(6) . . ?
O35 Mo18 O45 95.8(5) . . ?
O51 Mo18 O60 98.4(6) . . ?
O35 Mo18 O60 154.6(5) . . ?
O45 Mo18 O60 86.0(5) . . ?
O51 Mo18 O30 100.5(6) . . ?
O35 Mo18 O30 83.9(5) . . ?
O45 Mo18 O30 154.9(5) . . ?
O60 Mo18 O30 84.0(5) . . ?
O51 Mo18 O27 164.6(5) . . ?
O35 Mo18 O27 84.9(4) . . ?
O45 Mo18 O27 85.9(4) . . ?
O60 Mo18 O27 69.9(4) . . ?
O30 Mo18 O27 69.1(4) . . ?
O56 As2 O46 101.8(5) . . ?
O56 As2 O50 83.9(5) . . ?
O46 As2 O50 81.7(5) . . ?
O56 As2 As2 99.1(4) . 2_667 ?
O46 As2 As2 146.7(4) . 2_667 ?
O50 As2 As2 126.4(4) . 2_667 ?
O46 As2 Mo13 99.0(4) . . ?
As2 As2 Mo13 113.6(2) 2_667 . ?
O56 As2 Mo8 98.4(3) . . ?
As2 As2 Mo8 156.8(2) 2_667 . ?
Mo13 As2 Mo8 72.04(8) . . ?
O37 As3 O29 111.9(5) . . ?
O37 As3 O38 110.8(5) . . ?
O29 As3 O38 111.0(5) . . ?
O37 As3 O27 106.5(5) . . ?
O29 As3 O27 107.4(5) . . ?
O38 As3 O27 109.1(5) . . ?
O33 As4 O54 112.0(5) . . ?
O33 As4 O12 111.0(5) . . ?
O54 As4 O12 111.3(5) . . ?
O33 As4 O42 107.5(5) . . ?
O54 As4 O42 106.3(5) . . ?
O12 As4 O42 108.5(5) . . ?
Mo14 O5 Mo5 161.9(7) . . ?
As1 O7 Mo16 102.5(5) . . ?
As1 O7 Mo2 113.3(5) . . ?
Mo16 O7 Mo2 141.0(5) . . ?
Mo13 O9 Mo5 151.1(6) . . ?
As4 O12 Mo14 125.3(5) . . ?
As4 O12 Mo6 125.3(5) . . ?
Mo14 O12 Mo6 95.1(4) . . ?
Mo5 O13 Mo7 163.6(7) . . ?
Mo9 O14 Mo4 149.7(7) . . ?
Mo4 O15 Mo5 122.4(6) . . ?
Mo16 O16 Mo1 156.0(6) . . ?
Mo3 O17 Mo4 162.9(7) . . ?
Mo12 O22 Mo3 162.0(7) . . ?
Mo12 O23 Mo2 120.9(6) . . ?
Mo17 O25 Mo3 156.0(6) . . ?
Mo11 O26 Mo4 157.0(7) . . ?
As3 O27 Mo16 123.5(5) . . ?
As3 O27 Mo18 121.6(5) . . ?
Mo16 O27 Mo18 91.7(4) . . ?
As3 O27 Mo17 122.9(5) . . ?
Mo16 O27 Mo17 97.7(4) . . ?
Mo18 O27 Mo17 91.0(4) . . ?
Mo13 O28 Mo9 120.8(5) . . ?
As3 O29 Mo3 126.5(6) . . ?
As3 O29 Mo7 125.5(6) . . ?
Mo3 O29 Mo7 93.5(4) . . ?
Mo17 O30 Mo18 125.9(7) . . ?
Mo8 O31 Mo9 122.1(6) . . ?
As1 O32 Mo16 100.0(6) . . ?
As1 O32 Mo17 98.6(6) . . ?
Mo16 O32 Mo17 116.9(6) . . ?
As4 O33 Mo4 125.4(5) . . ?
As4 O33 Mo5 126.6(5) . . ?
Mo4 O33 Mo5 93.7(4) . . ?
Mo15 O34 Mo1 124.0(6) . . ?
Mo18 O35 Mo7 146.4(6) . . ?
Mo3 O36 Mo7 122.0(6) . . ?
As3 O37 Mo15 125.3(5) . . ?
As3 O37 Mo1 126.2(5) . . ?
Mo15 O37 Mo1 94.1(4) . . ?
As3 O38 Mo2 126.7(6) . . ?
As3 O38 Mo12 125.4(5) . . ?
Mo2 O38 Mo12 95.4(4) . . ?
Mo6 O39 Mo10 155.9(7) . . ?
Mo14 O40 Mo6 121.3(6) . . ?
Mo12 O41 Mo11 157.9(7) . . ?
As4 O42 Mo9 123.1(5) . . ?
As4 O42 Mo8 124.2(5) . . ?
Mo9 O42 Mo8 92.0(3) . . ?
As4 O42 Mo13 121.9(5) . . ?
Mo9 O42 Mo13 91.6(3) . . ?
Mo8 O42 Mo13 95.4(4) . . ?
Mo10 O43 Na1 175.8(7) . 2_577 ?
Mo6 O44 Mo1 162.3(6) . . ?
Mo18 O45 Mo15 145.1(6) . . ?
As2 O46 Mo8 99.5(5) . . ?
As2 O46 Mo6 110.3(5) . . ?
Mo8 O46 Mo6 146.2(6) . . ?
As1 O47 Mo17 103.8(5) . . ?
As1 O47 Mo12 111.9(5) . . ?
Mo17 O47 Mo12 140.1(6) . . ?
Mo10 O48 Mo11 122.5(6) . . ?
Mo10 O48 Na1 113.8(5) . . ?
Mo11 O48 Na1 123.4(6) . . ?
Mo7 O49 Mo15 158.4(7) . . ?
Mo8 O50 As2 97.0(5) . . ?
Mo8 O50 Mo13 118.4(5) . . ?
As2 O50 Mo13 93.0(5) . . ?
Mo9 O53 Mo11 145.7(6) . . ?
As4 O54 Mo11 125.1(6) . . ?
As4 O54 Mo10 125.1(6) . . ?
Mo11 O54 Mo10 94.7(4) . . ?
Mo14 O55 Mo15 163.1(7) . . ?
As2 O56 Mo13 102.3(5) . . ?
As2 O56 Mo14 109.6(5) . . ?
Mo13 O56 Mo14 145.1(6) . . ?
Mo2 O58 Mo10 158.9(7) . . ?
Mo16 O60 Mo18 123.9(6) . . ?
Mo8 O61 Mo10 151.3(6) . . ?
Mo2 O62 Mo1 160.7(7) . . ?
N9 Cu1 N11 175.5(9) . . ?
C10 N11 C12 106.3(19) . . ?
C10 N11 Cu1 125.0(16) . . ?
C12 N11 Cu1 128.8(16) . . ?
C11 N12 C10 108(2) . . ?
C9 N9 C7 102(3) . . ?
C9 N9 Cu1 130(2) . . ?
C7 N9 Cu1 127(2) . . ?
C8 N10 C9 106(3) . . ?
C8 C7 N9 111(3) . . ?
C8 C7 H7 124.3 . . ?
N9 C7 H7 124.3 . . ?
N9 C9 N10 113(3) . . ?
N9 C9 H9 123.4 . . ?
N10 C9 H9 123.4 . . ?
N12 C11 C12 109(2) . . ?
N12 C11 H11 125.7 . . ?
C12 C11 H11 125.7 . . ?
N11 C10 N12 109(2) . . ?
N11 C10 H10 125.7 . . ?
N12 C10 H10 125.6 . . ?
C11 C12 N11 109(2) . . ?
C11 C12 H12 125.6 . . ?
N11 C12 H12 125.7 . . ?
C7 C8 N10 107(3) . . ?
C7 C8 H8 126.7 . . ?
N10 C8 H8 126.8 . . ?
N4 Cu2 N2 179.0(8) . . ?
C21 N4 C19 103.3(16) . . ?
C21 N4 Cu2 127.2(13) . . ?
C19 N4 Cu2 129.4(14) . . ?
C24 N2 C23 106.4(17) . . ?
C24 N2 Cu2 126.5(15) . . ?
C23 N2 Cu2 126.7(14) . . ?
C22 N1 C24 107.5(18) . . ?
C21 N3 C20 108.8(16) . . ?
C19 C20 N3 104(2) . . ?
C19 C20 H20 128.1 . . ?
N3 C20 H20 128.2 . . ?
C23 C22 N1 108(2) . . ?
C23 C22 H22 126.1 . . ?
N1 C22 H22 126.0 . . ?
C20 C19 N4 113(2) . . ?
C20 C19 H19 123.7 . . ?
N4 C19 H19 123.6 . . ?
N2 C24 N1 110.2(19) . . ?
N2 C24 H24 124.8 . . ?
N1 C24 H24 124.9 . . ?
N4 C21 N3 111.3(16) . . ?
N4 C21 H21 124.3 . . ?
N3 C21 H21 124.4 . . ?
C22 C23 N2 107.4(19) . . ?
C22 C23 H23 126.3 . . ?
N2 C23 H23 126.3 . . ?
N5 Na1 N7 171.6(12) . . ?
N5 Na1 O43 88.4(8) . 2_577 ?
N7 Na1 O43 85.4(9) . 2_577 ?
N5 Na1 O48 86.9(8) . . ?
N7 Na1 O48 95.3(9) . . ?
O43 Na1 O48 146.3(5) 2_577 . ?
N5 Na1 Na1 83.1(8) . 2_577 ?
N7 Na1 Na1 88.7(9) . 2_577 ?
O43 Na1 Na1 55.0(3) 2_577 2_577 ?
O48 Na1 Na1 91.3(4) . 2_577 ?
C14 N6 C15 106(2) . . ?
C15 N5 C13 102(2) . . ?
C15 N5 Na1 122(2) . . ?
C13 N5 Na1 133.9(19) . . ?
N6 C15 N5 108(3) . . ?
N6 C15 H15 125.9 . . ?
N5 C15 H15 125.8 . . ?
C13 C14 N6 112(2) . . ?
C13 C14 H14 124.1 . . ?
N6 C14 H14 124.2 . . ?
C14 C13 N5 111(2) . . ?
C14 C13 H13 124.5 . . ?
N5 C13 H13 124.2 . . ?
H2WA O2W H2WB 120.0 . . ?
H1WA O1W H1WB 120.0 . . ?
C3 N1B C2 112(3) . . ?
C3 N1C C1 107(3) . . ?
N1B C3 N1C 109(3) . . ?
N1B C3 H3 125.4 . . ?
N1C C3 H3 125.4 . . ?
C1 C2 N1B 107(4) . . ?
C1 C2 H2 126.8 . . ?
N1B C2 H2 126.7 . . ?
C2 C1 N1C 105(4) . . ?
C2 C1 H1 127.3 . . ?
N1C C1 H1 127.5 . . ?
N1G C6 N1D 108.0 . . ?
N1G C6 H6 126.1 . . ?
N1D C6 H6 125.9 . . ?
C6 N1G C5 108.0 . . ?
C4 C5 N1G 108.0 . . ?
C4 C5 H5 126.0 . . ?
N1G C5 H5 126.0 . . ?
C5 C4 N1D 108.0 . . ?
C5 C4 H4 126.0 . . ?
N1D C4 H4 126.0 . . ?
C6 N1D C4 108.0 . . ?
C16 N7 C18 108.0 . . ?
C16 N7 Na1 105.0(18) . . ?
C18 N7 Na1 146.9(18) . . ?
C17 C18 N7 108.0 . . ?
C17 C18 H18 126.0 . . ?
N7 C18 H18 126.0 . . ?
C18 C17 N8 108.0 . . ?
C18 C17 H17 126.0 . . ?
N8 C17 H17 126.0 . . ?
C16 N8 C17 108.0 . . ?
N8 C16 N7 108.0 . . ?
N8 C16 H16 126.0 . . ?
N7 C16 H16 126.0 . . ?
O47 As1 O7 102.7(5) . . ?
O47 As1 O32 84.0(5) . . ?
O7 As1 O32 82.7(5) . . ?
O7 As1 Mo17 98.9(4) . . ?
O47 As1 Mo16 99.7(4) . . ?
Mo17 As1 Mo16 71.42(10) . . ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
O2W H2WA O51 0.85 1.98 2.82(2) 168.5 2_666
O2W H2WB N1B 0.85 1.90 2.66(3) 148.7 .
O1W H1WA O28 0.85 2.23 3.08(2) 179.1 2_666
O1W H1WB N6 0.85 2.31 2.82(3) 118.2 1_544
O1W H1WB O11 0.85 2.44 2.91(2) 115.2 2_566

_diffrn_measured_fraction_theta_max 0.987
_diffrn_reflns_theta_full        25.00
_diffrn_measured_fraction_theta_full 0.987
_refine_diff_density_max         5.020
_refine_diff_density_min         -3.119
_refine_diff_density_rms         0.317
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_aa
_database_code_depnum_ccdc_archive 'CCDC 1521984'
_audit_update_record             
;
2016-12-11 deposited with the CCDC.
2017-03-21 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'C144 H144 As12 Cu36 Mo108 N216 O372'
_chemical_formula_sum            'C144 H144 As12 Cu36 Mo108 N216 O372'
_chemical_formula_weight         24400.75

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           trigonal
_symmetry_space_group_name_H-M   ' R -3 c'
_symmetry_space_group_name_Hall  ' -R 3 2"c'
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'y, x, -z+1/2'
'-x, -x+y, -z+1/2'
'x-y, -y, -z+1/2'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'y+2/3, x+1/3, -z+5/6'
'-x+2/3, -x+y+1/3, -z+5/6'
'x-y+2/3, -y+1/3, -z+5/6'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'y+1/3, x+2/3, -z+7/6'
'-x+1/3, -x+y+2/3, -z+7/6'
'x-y+1/3, -y+2/3, -z+7/6'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-y, -x, z-1/2'
'x, x-y, z-1/2'
'-x+y, y, z-1/2'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'-y+2/3, -x+1/3, z-1/6'
'x+2/3, x-y+1/3, z-1/6'
'-x+y+2/3, y+1/3, z-1/6'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, x+2/3, -z+2/3'
'-y+1/3, -x+2/3, z+1/6'
'x+1/3, x-y+2/3, z+1/6'
'-x+y+1/3, y+2/3, z+1/6'

_cell_length_a                   22.034(13)
_cell_length_b                   22.034(13)
_cell_length_c                   34.773(16)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_volume                     14620(14)
_cell_formula_units_Z            1
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    3437
_cell_measurement_theta_min      1.58
_cell_measurement_theta_max      28.26

_exptl_crystal_description       block
_exptl_crystal_colour            blue
_exptl_crystal_size_max          0.22
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.18
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    2.771
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             11472
_exptl_absorpt_coefficient_mu    4.290
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.4521
_exptl_absorpt_correction_T_max  0.5123
_exptl_absorpt_process_details   SADABS

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Bruker Smart APEX CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            28133
_diffrn_reflns_av_R_equivalents  0.0307
_diffrn_reflns_av_sigmaI/netI    0.0158
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_h_max       26
_diffrn_reflns_limit_k_min       -26
_diffrn_reflns_limit_k_max       26
_diffrn_reflns_limit_l_min       -41
_diffrn_reflns_limit_l_max       39
_diffrn_reflns_theta_min         1.58
_diffrn_reflns_theta_max         25.38
_reflns_number_total             2937
_reflns_number_gt                2439
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    SHELXP-97
_computing_publication_material  SHELXTL

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.1032P)²+1296.6532P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    mixed
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         2937
_refine_ls_number_parameters     272
_refine_ls_number_restraints     89
_refine_ls_R_factor_all          0.0891
_refine_ls_R_factor_gt           0.0717
_refine_ls_wR_factor_ref         0.2128
_refine_ls_wR_factor_gt          0.1827
_refine_ls_goodness_of_fit_ref   1.070
_refine_ls_restrained_S_all      1.069
_refine_ls_shift/su_max          0.005
_refine_ls_shift/su_mean         0.001

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
C1 C 0.1486(12) 0.3592(11) 0.9673(5) 0.076(6) Uani 1 1 d . . .
H1 H 0.1399 0.3429 0.9421 0.091 Uiso 1 1 calc R . .
C2 C 0.1898(13) 0.4252(11) 0.9788(5) 0.085(7) Uani 1 1 d . . .
H2 H 0.2137 0.4642 0.9630 0.101 Uiso 1 1 calc R . .
C3 C 0.9260(16) 0.2330(18) 0.1842(7) 0.122(10) Uani 1 1 d U . .
H3 H 0.9090 0.1922 0.1987 0.16(12) Uiso 1 1 calc R . .
C4 C 0.9423(18) 0.295(2) 0.1973(7) 0.134(11) Uani 1 1 d U . .
H4 H 0.9379 0.3061 0.2225 0.16(12) Uiso 1 1 calc R . .
Cu1 Cu 0.13410(15) 0.3333 1.0833 0.0589(7) Uani 1 2 d S . .
Cu2 Cu 0.9836(2) 0.3333 0.0833 0.0970(14) Uani 1 2 d S . .
Mo1 Mo -0.04208(6) -0.10338(6) 0.14342(3) 0.0358(3) Uani 1 1 d . . .
Mo2 Mo -0.02913(6) 0.14329(5) 0.05200(3) 0.0325(3) Uani 1 1 d U . .
Mo3 Mo 0.14344(6) 0.17114(5) 0.05676(3) 0.0356(3) Uani 1 1 d U . .
N1 N 0.9384(10) 0.2387(10) 0.1459(5) 0.089(5) Uani 1 1 d . . .
N2 N 0.9600(9) 0.3023(8) 0.1338(4) 0.069(4) Uani 1 1 d . . .
N3 N 0.9677(15) 0.3405(14) 0.1659(7) 0.127(8) Uani 1 1 d U . .
N4 N 0.1210(11) 0.3194(9) 1.0007(4) 0.082(5) Uani 1 1 d . . .
N5 N 0.1475(7) 0.3604(6) 1.0311(4) 0.052(3) Uani 1 1 d . . .
N6 N 0.1903(10) 0.4247(8) 1.0181(4) 0.079(5) Uani 1 1 d . . .
O1 O -0.0633(5) -0.1649(5) 0.1779(2) 0.045(2) Uani 1 1 d . . .
O2 O -0.0800(5) -0.0501(5) 0.1669(2) 0.0366(19) Uani 1 1 d . . .
O7 O 0.1201(4) 0.1365(4) 0.1094(2) 0.0306(17) Uani 1 1 d . A .
O8 O 0.2071(5) 0.2508(5) 0.0667(3) 0.053(3) Uani 1 1 d . A .
O10 O -0.0307(4) 0.1126(4) 0.1090(2) 0.0312(17) Uani 1 1 d . . .
O9 O 0.0722(5) 0.1975(5) 0.0576(3) 0.0472(11) Uani 1 1 d U A 3
O11 O -0.1296(5) 0.0745(6) 0.0598(3) 0.0533(13) Uani 1 1 d U A 3
O12 O -0.0411(6) 0.2093(5) 0.0649(3) 0.051(3) Uani 1 1 d . A .
O13 O -0.0301(7) 0.1514(6) -0.0008(3) 0.056(3) Uani 1 1 d . . .
As1 As 0.0000 0.0000 0.05790(5) 0.0201(4) Uani 1 3 d SU . .
O3 O 0.0000 0.0000 0.1071(3) 0.024(3) Uani 1 3 d SU . .
O4A O -0.028(3) -0.073(3) 0.046(2) 0.014(5) Uani 0.179(6) 1 d PU . 1
O5A O 0.093(3) 0.058(3) 0.0401(12) 0.008(6) Uani 0.179(6) 1 d PU . 1
O6A O -0.054(4) 0.031(4) 0.050(2) 0.020(4) Uani 0.179(6) 1 d PU . 1
O4B O 0.030(6) 0.082(8) 0.045(3) 0.016(5) Uani 0.154(6) 1 d PU . 2
O5B O -0.091(4) -0.058(4) 0.041(4) 0.011(6) Uani 0.154(6) 1 d PU . 2
O6B O 0.050(5) -0.027(4) 0.038(3) 0.014(4) Uani 0.154(6) 1 d PU . 2


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
C1 C2 1.33(3) . ?
C1 N4 1.40(3) . ?
C1 H1 0.9300 . ?
C2 N6 1.37(2) . ?
C2 H2 0.9300 . ?
C3 C4 1.30(4) . ?
C3 N1 1.35(3) . ?
C3 H3 0.9300 . ?
C4 N3 1.40(4) . ?
C4 H4 0.9300 . ?
Cu1 N5 1.887(13) 18_556 ?
Cu1 N5 1.887(13) . ?
Cu2 N2 1.860(15) 18_554 ?
Cu2 N2 1.860(15) . ?
Mo1 O1 1.691(8) . ?
Mo1 O10 1.803(8) 2 ?
Mo1 O7 1.918(8) 3 ?
Mo1 O2 1.930(9) . ?
Mo1 O2 2.032(9) 2 ?
Mo1 O3 2.352(7) . ?
Mo2 O12 1.665(9) . ?
Mo2 O13 1.845(9) . ?
Mo2 O9 1.945(10) . ?
Mo2 O11 1.979(10) . ?
Mo2 O10 2.089(8) . ?
Mo2 O5A 2.17(5) 2 ?
Mo2 O5B 2.22(8) 3 ?
Mo2 O6A 2.26(8) . ?
Mo2 O4B 2.32(12) . ?
Mo2 O4A 2.39(7) 3 ?
Mo2 O6B 2.39(9) 2 ?
Mo3 O8 1.646(9) . ?
Mo3 O9 1.926(10) . ?
Mo3 O7 1.949(8) . ?
Mo3 O13 1.958(9) 20 ?
Mo3 O11 1.965(11) 3 ?
Mo3 O5B 2.24(10) 3 ?
Mo3 O5A 2.25(5) . ?
Mo3 O6A 2.25(7) 3 ?
Mo3 O4B 2.31(14) . ?
Mo3 O4A 2.45(6) 2 ?
Mo3 O6B 2.45(7) 2 ?
N1 N2 1.30(2) . ?
N2 N3 1.36(3) . ?
N4 N5 1.324(18) . ?
N5 N6 1.33(2) . ?
O2 Mo1 2.032(9) 3 ?
O7 Mo1 1.918(8) 2 ?
O10 Mo1 1.803(8) 3 ?
O11 Mo3 1.965(11) 2 ?
O13 Mo3 1.958(9) 21 ?
As1 O4A 1.46(7) 2 ?
As1 O4A 1.46(7) 3 ?
As1 O4A 1.46(7) . ?
As1 O4B 1.64(14) 2 ?
As1 O4B 1.64(14) . ?
As1 O4B 1.64(14) 3 ?
As1 O6B 1.64(14) . ?
As1 O6B 1.64(14) 3 ?
As1 O6B 1.64(14) 2 ?
As1 O6A 1.66(9) 2 ?
As1 O6A 1.66(9) . ?
As1 O6A 1.66(9) 3 ?
O3 Mo1 2.352(7) 2 ?
O3 Mo1 2.352(7) 3 ?
O4A O6A 0.27(11) 2 ?
O4A O5A 0.45(6) 3 ?
O4A Mo2 2.39(7) 2 ?
O4A Mo3 2.45(6) 3 ?
O5A O6A 0.37(10) 3 ?
O5A O4A 0.45(7) 2 ?
O5A Mo2 2.17(5) 3 ?
O6A O4A 0.27(11) 3 ?
O6A O5A 0.37(10) 2 ?
O6A Mo3 2.25(7) 2 ?
O4B O5B 0.24(11) 3 ?
O4B O6B 0.28(12) 2 ?
O5B O4B 0.24(11) 2 ?
O5B O6B 0.30(9) 3 ?
O5B Mo2 2.22(8) 2 ?
O5B Mo3 2.24(10) 2 ?
O6B O4B 0.28(12) 3 ?
O6B O5B 0.30(9) 2 ?
O6B Mo2 2.39(9) 3 ?
O6B Mo3 2.45(7) 3 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
C2 C1 N4 106.2(14) . . ?
C2 C1 H1 126.9 . . ?
N4 C1 H1 126.9 . . ?
C1 C2 N6 107.2(18) . . ?
C1 C2 H2 126.4 . . ?
N6 C2 H2 126.4 . . ?
C4 C3 N1 108(3) . . ?
C4 C3 H3 126.0 . . ?
N1 C3 H3 126.0 . . ?
C3 C4 N3 106(2) . . ?
C3 C4 H4 126.8 . . ?
N3 C4 H4 126.8 . . ?
N5 Cu1 N5 179.7(9) 18_556 . ?
N2 Cu2 N2 169.1(11) 18_554 . ?
O1 Mo1 O10 104.7(4) . 2 ?
O1 Mo1 O7 103.1(4) . 3 ?
O10 Mo1 O7 89.7(3) 2 3 ?
O1 Mo1 O2 99.0(4) . . ?
O10 Mo1 O2 92.8(4) 2 . ?
O7 Mo1 O2 156.3(3) 3 . ?
O1 Mo1 O2 96.8(4) . 2 ?
O10 Mo1 O2 158.4(3) 2 2 ?
O7 Mo1 O2 84.3(3) 3 2 ?
O2 Mo1 O2 84.8(5) . 2 ?
O1 Mo1 O3 166.9(4) . . ?
O10 Mo1 O3 86.7(3) 2 . ?
O7 Mo1 O3 82.9(3) 3 . ?
O2 Mo1 O3 73.7(3) . . ?
O2 Mo1 O3 72.0(3) 2 . ?
O12 Mo2 O13 99.7(4) . . ?
O12 Mo2 O9 94.1(5) . . ?
O13 Mo2 O9 96.1(5) . . ?
O12 Mo2 O11 91.5(5) . . ?
O13 Mo2 O11 98.5(5) . . ?
O9 Mo2 O11 163.3(4) . . ?
O12 Mo2 O10 92.5(4) . . ?
O13 Mo2 O10 167.4(4) . . ?
O9 Mo2 O10 86.1(4) . . ?
O11 Mo2 O10 77.9(4) . . ?
O12 Mo2 O5A 157.2(16) . 2 ?
O13 Mo2 O5A 84.5(11) . 2 ?
O9 Mo2 O5A 107.8(15) . 2 ?
O11 Mo2 O5A 65.7(16) . 2 ?
O10 Mo2 O5A 83.0(11) . 2 ?
O12 Mo2 O5B 155(3) . 3 ?
O13 Mo2 O5B 85(3) . 3 ?
O9 Mo2 O5B 61(3) . 3 ?
O11 Mo2 O5B 112(2) . 3 ?
O10 Mo2 O5B 85(3) . 3 ?
O5A Mo2 O5B 47(3) 2 3 ?
O12 Mo2 O6A 155.8(17) . . ?
O13 Mo2 O6A 93(2) . . ?
O9 Mo2 O6A 105(2) . . ?
O11 Mo2 O6A 66.4(19) . . ?
O10 Mo2 O6A 74(2) . . ?
O5A Mo2 O6A 9(2) 2 . ?
O5B Mo2 O6A 46(3) 3 . ?
O12 Mo2 O4B 157(4) . . ?
O13 Mo2 O4B 90(2) . . ?
O9 Mo2 O4B 64(4) . . ?
O11 Mo2 O4B 108(3) . . ?
O10 Mo2 O4B 80.1(19) . . ?
O5A Mo2 O4B 44(4) 2 . ?
O5B Mo2 O4B 6(3) 3 . ?
O6A Mo2 O4B 42(4) . . ?
O12 Mo2 O4A 161.6(15) . 3 ?
O13 Mo2 O4A 91(2) . 3 ?
O9 Mo2 O4A 99.7(15) . 3 ?
O11 Mo2 O4A 71.9(14) . 3 ?
O10 Mo2 O4A 76(2) . 3 ?
O5A Mo2 O4A 9.9(18) 2 3 ?
O5B Mo2 O4A 40(2) 3 3 ?
O6A Mo2 O4A 6(3) . 3 ?
O4B Mo2 O4A 36(4) . 3 ?
O12 Mo2 O6B 161(2) . 2 ?
O13 Mo2 O6B 84(3) . 2 ?
O9 Mo2 O6B 67(2) . 2 ?
O11 Mo2 O6B 106(2) . 2 ?
O10 Mo2 O6B 86(3) . 2 ?
O5A Mo2 O6B 41(3) 2 2 ?
O5B Mo2 O6B 6(3) 3 2 ?
O6A Mo2 O6B 40(3) . 2 ?
O4B Mo2 O6B 7(3) . 2 ?
O4A Mo2 O6B 34(3) 3 2 ?
O8 Mo3 O9 93.6(5) . . ?
O8 Mo3 O7 97.9(4) . . ?
O9 Mo3 O7 90.4(4) . . ?
O8 Mo3 O13 96.0(4) . 20 ?
O9 Mo3 O13 91.1(5) . 20 ?
O7 Mo3 O13 165.8(4) . 20 ?
O8 Mo3 O11 94.0(5) . 3 ?
O9 Mo3 O11 170.4(4) . 3 ?
O7 Mo3 O11 82.9(4) . 3 ?
O13 Mo3 O11 93.8(5) 20 3 ?
O8 Mo3 O5B 154.2(19) . 3 ?
O9 Mo3 O5B 61(2) . 3 ?
O7 Mo3 O5B 87(3) . 3 ?
O13 Mo3 O5B 81(3) 20 3 ?
O11 Mo3 O5B 111.7(19) 3 3 ?
O8 Mo3 O5A 157.6(14) . . ?
O9 Mo3 O5A 108.5(14) . . ?
O7 Mo3 O5A 85.4(10) . . ?
O13 Mo3 O5A 80.7(11) 20 . ?
O11 Mo3 O5A 64.3(14) 3 . ?
O5B Mo3 O5A 48(2) 3 . ?
O8 Mo3 O6A 160(2) . 3 ?
O9 Mo3 O6A 105(2) . 3 ?
O7 Mo3 O6A 77(2) . 3 ?
O13 Mo3 O6A 89(2) 20 3 ?
O11 Mo3 O6A 67(2) 3 3 ?
O5B Mo3 O6A 45(3) 3 3 ?
O5A Mo3 O6A 9(3) . 3 ?
O8 Mo3 O4B 158(3) . . ?
O9 Mo3 O4B 64(3) . . ?
O7 Mo3 O4B 82.3(19) . . ?
O13 Mo3 O4B 86(2) 20 . ?
O11 Mo3 O4B 108(3) 3 . ?
O5B Mo3 O4B 6(3) 3 . ?
O5A Mo3 O4B 44(4) . . ?
O6A Mo3 O4B 41(4) 3 . ?
O8 Mo3 O4A 164.6(15) . 2 ?
O9 Mo3 O4A 101.3(16) . 2 ?
O7 Mo3 O4A 78(2) . 2 ?
O13 Mo3 O4A 87(2) 20 2 ?
O11 Mo3 O4A 70.7(15) 3 2 ?
O5B Mo3 O4A 41(2) 3 2 ?
O5A Mo3 O4A 9.8(19) . 2 ?
O6A Mo3 O4A 4(3) 3 2 ?
O4B Mo3 O4A 37(4) . 2 ?
O8 Mo3 O6B 159(3) . 2 ?
O9 Mo3 O6B 66(2) . 2 ?
O7 Mo3 O6B 88(3) . 2 ?
O13 Mo3 O6B 80(3) 20 2 ?
O11 Mo3 O6B 107(3) 3 2 ?
O5B Mo3 O6B 5(3) 3 2 ?
O5A Mo3 O6B 42(3) . 2 ?
O6A Mo3 O6B 40(3) 3 2 ?
O4B Mo3 O6B 6(3) . 2 ?
O4A Mo3 O6B 36(3) 2 2 ?
N2 N1 C3 112(2) . . ?
N1 N2 N3 105.4(18) . . ?
N1 N2 Cu2 125.9(13) . . ?
N3 N2 Cu2 128.5(16) . . ?
N2 N3 C4 108(2) . . ?
N5 N4 C1 109.4(15) . . ?
N4 N5 N6 106.9(14) . . ?
N4 N5 Cu1 127.4(11) . . ?
N6 N5 Cu1 125.5(10) . . ?
N5 N6 C2 110.2(15) . . ?
Mo1 O2 Mo1 120.3(4) . 3 ?
Mo1 O7 Mo3 144.8(4) 2 . ?
Mo1 O10 Mo2 147.9(4) 3 . ?
Mo3 O9 Mo2 132.2(5) . . ?
Mo3 O11 Mo2 124.9(6) 2 . ?
Mo2 O13 Mo3 168.0(5) . 21 ?
O4A As1 O4A 113(3) 2 3 ?
O4A As1 O4A 113(3) 2 . ?
O4A As1 O4A 113(3) 3 . ?
O4A As1 O4B 149(5) 2 2 ?
O4A As1 O4B 59(4) 3 2 ?
O4A As1 O4B 56(4) . 2 ?
O4A As1 O4B 59(4) 2 . ?
O4A As1 O4B 56(4) 3 . ?
O4A As1 O4B 149(5) . . ?
O4B As1 O4B 113(3) 2 . ?
O4A As1 O4B 56(4) 2 3 ?
O4A As1 O4B 149(5) 3 3 ?
O4A As1 O4B 59(4) . 3 ?
O4B As1 O4B 113(3) 2 3 ?
O4B As1 O4B 113(3) . 3 ?
O4A As1 O6B 54(4) 2 . ?
O4A As1 O6B 139(4) 3 . ?
O4A As1 O6B 59(4) . . ?
O4B As1 O6B 110(5) 2 . ?
O4B As1 O6B 108(5) . . ?
O4B As1 O6B 10(4) 3 . ?
O4A As1 O6B 139(4) 2 3 ?
O4A As1 O6B 59(4) 3 3 ?
O4A As1 O6B 54(4) . 3 ?
O4B As1 O6B 10(4) 2 3 ?
O4B As1 O6B 110(5) . 3 ?
O4B As1 O6B 108(5) 3 3 ?
O6B As1 O6B 103(3) . 3 ?
O4A As1 O6B 59(4) 2 2 ?
O4A As1 O6B 54(4) 3 2 ?
O4A As1 O6B 139(4) . 2 ?
O4B As1 O6B 108(5) 2 2 ?
O4B As1 O6B 10(4) . 2 ?
O4B As1 O6B 110(5) 3 2 ?
O6B As1 O6B 103(3) . 2 ?
O6B As1 O6B 103(3) 3 2 ?
O4A As1 O6A 113(5) 2 2 ?
O4A As1 O6A 117(5) 3 2 ?
O4A As1 O6A 6(5) . 2 ?
O4B As1 O6A 59(4) 2 2 ?
O4B As1 O6A 155(5) . 2 ?
O4B As1 O6A 58(4) 3 2 ?
O6B As1 O6A 59(4) . 2 ?
O6B As1 O6A 58(4) 3 2 ?
O6B As1 O6A 145(3) 2 2 ?
O4A As1 O6A 117(5) 2 . ?
O4A As1 O6A 6(5) 3 . ?
O4A As1 O6A 113(5) . . ?
O4B As1 O6A 58(4) 2 . ?
O4B As1 O6A 59(4) . . ?
O4B As1 O6A 155(5) 3 . ?
O6B As1 O6A 145(3) . . ?
O6B As1 O6A 59(4) 3 . ?
O6B As1 O6A 58(4) 2 . ?
O6A As1 O6A 117.0(15) 2 . ?
O4A As1 O6A 6(5) 2 3 ?
O4A As1 O6A 113(5) 3 3 ?
O4A As1 O6A 117(5) . 3 ?
O4B As1 O6A 155(5) 2 3 ?
O4B As1 O6A 58(4) . 3 ?
O4B As1 O6A 59(4) 3 3 ?
O6B As1 O6A 58(4) . 3 ?
O6B As1 O6A 145(3) 3 3 ?
O6B As1 O6A 59(4) 2 3 ?
O6A As1 O6A 117.0(15) 2 3 ?
O6A As1 O6A 117.0(15) . 3 ?
As1 O3 Mo1 122.5(3) . 2 ?
As1 O3 Mo1 122.5(3) . 3 ?
Mo1 O3 Mo1 93.8(3) 2 3 ?
As1 O3 Mo1 122.5(3) . . ?
Mo1 O3 Mo1 93.8(3) 2 . ?
Mo1 O3 Mo1 93.8(3) 3 . ?
O6A O4A O5A 59(10) 2 3 ?
O6A O4A As1 133(10) 2 . ?
O5A O4A As1 167(10) 3 . ?
O6A O4A Mo2 56(10) 2 2 ?
O5A O4A Mo2 56(9) 3 2 ?
As1 O4A Mo2 132(4) . 2 ?
O6A O4A Mo3 43(10) 2 3 ?
O5A O4A Mo3 58(10) 3 3 ?
As1 O4A Mo3 126(4) . 3 ?
Mo2 O4A Mo3 92.4(19) 2 3 ?
O6A O5A O4A 39(10) 3 2 ?
O6A O5A As1 46(10) 3 . ?
O4A O5A As1 10(10) 2 . ?
O6A O5A Mo2 96(10) 3 3 ?
O4A O5A Mo2 114(10) 2 3 ?
As1 O5A Mo2 120(2) . 3 ?
O6A O5A Mo3 85(10) 3 . ?
O4A O5A Mo3 112(10) 2 . ?
As1 O5A Mo3 115.2(19) . . ?
Mo2 O5A Mo3 105(3) 3 . ?
O4A O6A O5A 83(10) 3 2 ?
O4A O6A As1 40(10) 3 . ?
O5A O6A As1 125(10) 2 . ?
O4A O6A Mo3 132(10) 3 2 ?
O5A O6A Mo3 85(10) 2 2 ?
As1 O6A Mo3 127(4) . 2 ?
O4A O6A Mo2 118(10) 3 . ?
O5A O6A Mo2 71(10) 2 . ?
As1 O6A Mo2 128(4) . . ?
Mo3 O6A Mo2 102(3) 2 . ?
O5B O4B O6B 72(10) 3 2 ?
O5B O4B As1 157(10) 3 . ?
O6B O4B As1 86(10) 2 . ?
O5B O4B Mo3 69(10) 3 . ?
O6B O4B Mo3 118(10) 2 . ?
As1 O4B Mo3 125(4) . . ?
O5B O4B Mo2 63(10) 3 . ?
O6B O4B Mo2 104(10) 2 . ?
As1 O4B Mo2 125(5) . . ?
Mo3 O4B Mo2 100(6) . . ?
O4B O5B O6B 60(10) 2 3 ?
O4B O5B As1 20(10) 2 . ?
O6B O5B As1 40(10) 3 . ?
O4B O5B Mo2 112(10) 2 2 ?
O6B O5B Mo2 123(10) 3 2 ?
As1 O5B Mo2 120(4) . 2 ?
O4B O5B Mo3 106(10) 2 2 ?
O6B O5B Mo3 133(10) 3 2 ?
As1 O5B Mo3 117(5) . 2 ?
Mo2 O5B Mo3 105(4) 2 2 ?
O4B O6B O5B 49(10) 3 2 ?
O4B O6B As1 86(10) 3 . ?
O5B O6B As1 134(10) 2 . ?
O4B O6B Mo2 70(10) 3 3 ?
O5B O6B Mo2 51(10) 2 3 ?
As1 O6B Mo2 121(5) . 3 ?
O4B O6B Mo3 56(10) 3 3 ?
O5B O6B Mo3 42(10) 2 3 ?
As1 O6B Mo3 116(5) . 3 ?
Mo2 O6B Mo3 94(3) 3 3 ?

_diffrn_measured_fraction_theta_max 0.982
_diffrn_reflns_theta_full        25.38
_diffrn_measured_fraction_theta_full 0.982
_refine_diff_density_max         5.117
_refine_diff_density_min         -3.120
_refine_diff_density_rms         0.303
